Microstructure and Mechanical Property ... MICROSTRUCTURE AND MECHANICAL PROPERTY DEVELOPMENT IN...
Embed Size (px)
Transcript of Microstructure and Mechanical Property ... MICROSTRUCTURE AND MECHANICAL PROPERTY DEVELOPMENT IN...
MICROSTRUCTURE AND MECHANICAL PROPERTY DEVELOPMENT IN SUPERALLOY U72OLI
David Uhich Furrer and Hans-Jorg Fecht*
Ladish Co., Inc., PO Box 8902, Cudahy, WI 53 110, USA *Universitat Ulm, Albert-Einstein-Allee 47, D-8908 1 Uhn, Germany
Superalloy Udimet 720LITM has been studied and implemented into many production applications. [1,2] Further work has been conducted to assess the nature of the microstructural evolution and mechanical properly development in this alloy. This effort is focussed on thermal processing cycles to tailor gamma-prime distribution and gram boundary morphologies, and subsequent mechanical properties. The results of this work have been compared to previous studies and assessed with regard to basic physical metallurgy understanding of the observed microstructure/property relationships. A new thermal processing route has been established which will allow for an optimmn balance in mechanical properties for this material for potential future applications.
A three-phased experimental program was undertaken to study U72OLI material. A laboratory phase was conducted on heat treated microspecimens. A property screening phase, which incorporated mechanical property test specimens to evaluate heat treatment cooling rates, was performed. A full scale forging demonstration and validation phase was also conducted to more completely assess the microstructure and mechanical property interactions in U72OLI.
Laboratory Heat Treat Studies
To study the microstructural evolution in superalloy U72OL1, laboratory experiments where performed to characterize the microstructure and phases present after various thermal treatments. Initial studies were performed on billet samples from both powder metallurgy (P/M) and cast and wrought (C&W) (i.e. ingot metallurgy) materials. Laboratory thermal treatment studies focused on both
N Udimet is a registered trademark of Special Metals Corporation.
subsolvus and supersolvus solution heat treatment cycles and aging treatments.
The specific chemistry for the U72OLI materials investigated in this program is listed in Table I. The gamma-prime solvus for the P/M and cast and wrought U72OLI billet material was determined to be 1155’C, and 1160°C respectively.
Table I. Chemistry of the U72OLI material studied (w?h). Cr co Ti Al MO W Zr C B Ni
P/M lb.26 14.73 5.05 2.50 3.01 1.27 0.036 0.023 0.018 Rem.
C&W 16.06 14.52 5.04 2.54 3.08 1.20 0.047 0.013 0.018 Rem.
Billet slices of each material were sectioned by wire electric discharge machining (EDM) to produce 12.7 x 12.7 x 25.4 mm heat treatment blocks, Holes 1.6 mm in diameter were drilled in the center of the 12.7 x 12.7 mm face to a depth of 12.7 mm for insertion of a friction fit sheathed thermocouple.
Solution heat treatment studies were performed on the heat treatment blocks with thermocouples attached. Controlled cooling at different cooling rates was achieved by imposing different cooling media, such as air, oil and water, and by wrapping the blocks with various layers of insulating media to retard cooling to simulate large -turbine disc-type components. An extensive matrix of heat treatment conditions were performed on the program samples, which included supersolvus and subsolvus solution cycles.
After solution heat treating, the samples were sectioned at the middle of the block, normal to the thermocouple hole for metallographic analysis and further aging studies. Aging studies were performed on select samples to determine the changes in phase types, quantities and morphologies.
415 Superalloys 2000
Edited by TM. Pollock, R.D. Kissinger, R.R. Bowman, K.A. Green, M. McLean, S. Olson, and J.J. Schh,
‘IMY (The Minerals, Metals & Materials Society), 2000
Propertv Screening Phase
In addition to the heat treated metallographic samples, laboratory test bar samples were processed, mechanically tested and characterized. These samples are similar to the smaller block samples outlined above, but are much longer in size to accommodate machining mechanical test specimens from them after laboratory heat treatment. These cooling-rate test bars also had thermocouples inserted into one end to allow measurement of the exact cooling rate profile the bars experienced during the imposed heat treatment cycle. These samples were used to evaluate the effects of solution heat treat cycle and cooling rate on final elevated temperature tensile and creep properties.
Both cast and wrought and powder metallurgy U72OLI were tested in this phase. Supersolvus solution treatments were performed to allow assessment of intermediate (P/M) and coarse (C&W) structures. Table II lists the processing conditions given to each series of test bars.
Table II. Solution heat treatment cycles used for the mechanical property screening test samples. All samples were given a 760°C/8hrs./AC + 649’C/24hrs./AC age treatment.
Full-Scale Faming Evaluation
The forging phase of this program was designed to develop and expand upon the microstructure I mechanical property relationships for P/M U72OLI material. C&W U72OLI
processed by a supersolvus solution cycle did not show a capability of developing a good balance of tensile and creep properties and was not pursued after the property screening phase.
For this effort, 229mm diameter by 132mm tall P/M U72OLI billet material was isothermally forged into a 427mm diameter x 38mm thick pancake material. The chemistry of this material is listed in Table III.
Table III. Chemistry of the P/M U72OLI billet material used for the full-scale forging efforts (wt.-%).
Cr Co Ti MO Al W Fe Zr 16.35 14.78 5.01 3.00 2.41 1.35 0.09 0.031
B C Mn Si Cu P S N2 0.017 0.021 co.02 co.06 0.02
Table IV. Aging cycles given to the full-scale forged samples.
Ape Cycle 1 Cycle 2 A 843°C/8hrs.fFAQ 76O”C/16hm./AC B 76O”Cf 16hrs.lAC - - C 649°C/24hrs./AC 760°C/1 Ghrs./AC
Laboratory Heat Treat Studies
Optical and electron microscopy was performed on the laboratory heat treat samples. Grain size, gamma-prime size and morphology, and grain boundary morphology features were fully characterized as functions of solution
$j 60 55 .f
50 40- 0 0 q
1140 1160 1160 Solution Temperature(C)
heat treatment temperature and cooling rate. The grain growth behavior of the powder metallurgy and ingot metallurgy materials are distinctly different. Figure 2 shows grain growth plots for both materials as a function of solution temperature.
Light and electron optic metallography performed on the laboratory heat treatment specimens revealed a strong cooling rate I gamma-prime size dependence. Figure 3 shows example photomicrographs, which show this correlation. Secondary gamma-prime size measurements were performed on carefully prepared scanning electron microscope specimens. Supplemental measurements were conducted on select samples using transmission electron microscopy. The TEM measurements confnmed the measurements performed by the SEM evaluation technique.
1400 G? g1200 .b .5000
+i f330 t?J 8 400
1000 1050 1100 1150 1200 SolutionTemperature
Figure 2. Plot of grain size as a function of solution heat treatment temperature for A) P/M and B) C&W U72OLI material.
The grain boundary morphology of supersolvus solution heat treated samples was seen to change as a function of cooling rate. Figure 4 shows photomicrographs of P/M U72OLI grain boundaries after two different cooling rates. All of the grain boundaries of supersolvus solution heat
treated material exhibited serrations. The faster the cooling rate, the smaller the amplitude and period of the serrations. Figure 5 shows a plot of serration morphology as a ftmction of cooling rate.
55 1.2 g 6 1
s 3 0.4 E '3 t
0 5 10 15
Cooling Rate Just Prior to Precipitation (Chc)
Figure 3. Photomicrographs of supersolvus solution heat treated P/M U72OLI samples cooled at A) 12.7”C/sec, B) 1.3“C/sec, C) O.lTC/sec, and D) a plot expressing gamma-prime size as a function of cooling rate.
4 / P /
Figure 4. Serrated grain boundary morphologies of P/M U72OLI material supersolvus solution treated and cooled at A) 12.7Wsec and B) 1.3Wsec. A and P represent the measurements taken to assess set-ration amplitude and period respectively.
’ - no Senation Applitude]
0 0.0 2.0 4.0 6.0 8.0 10.0 12.0 14.0
Cooling Rate From 1168 to 816% (C/Set)
boundary serration amplitude for supersolvus solution treated PiM U72OLI as a Figure function of cooling rate.
Electrolytic extractions were performed on all laboratory heat treatment samples to assess the formation of carbide and boride phases as a result of the various thermal treatments. Samples were evaluated in the solution heat treated as well as aged condition. The as-solution heat treated samples allowed an estimation of the M& and M3Bz phase solvus temperatures as being between 103O”C- 104O’C and 106O’C respectively.
The cast and wrought U72OLI material contained large primary carbides [l], whereas the powder metallurgy material only exh